1 NUKLEONIKA 2010;55(2): ORIGINAL PAPER Sorption of lead(ii) on copper(ii) and nickel-potassium hexacyanoferrates and magnetite-loaded resin from inorganic acid solutions Barbara Kubica Abstract. The sorption of Pb 2+ on the composite sorbent obtained by incorporating of copper(ii)-potassium hexacyanoferrate or nickel(ii)-potassium hexacyanoferrate and magnetite into sulphonated phenolic resin was studied. The sorption kinetics were performed in hydrochloric, nitric and sulphuric acid solutions in the concentrations range from 10 4 mol dm 3 to 1 mol dm 3. The distribution coefficients for the lead(ii) sorption on the sorbents in these conditions were determined. The highest K d values, more than 1000 cm 3 g 1, were obtained for composite sorbents CuNCFM from HCl, HNO 3 and H 2 SO 4 (range concentration ) and for CuNCF and NiNCF from HCl (range concentration ). Also, the lead(ii) sorption on the magnetite-loaded resin was performed. Key words: sorption Pb 2+ hexacyanoferrates composite sorbents distribution coefficient (K d ) Introduction B. Kubica The Henryk Niewodniczański Institute of Nuclear Physics, Polish Academy of Sciences, 152 Radzikowskiego Str., Kraków, Poland, Tel.: , Fax: , Received: 5 August 2009 Accepted: 3 November 2009 Since lead is expected to be a homologue of element 114, study on the sorption of its trace quantity can give some useful information on the behaviour of element 114 under the same conditions . The predicted ground state electron configuration of the atoms of element 114 is similar to that of lead . The theory [20, 22] predicts the so-called stability island, for superheavy elements where half-lives of their isotopes might be as long as several minutes and more. Until now, the isotopes of element 114 with the atomic masses of 287, 288, 289 and half-lives of 6, 2.8 and 30.4 s, respectively, have been synthesized  what indicates that the solution chemistry investigation of element 114 is feasible . The method of continuous on-line isolation of short-lived transactinide elements together with simultaneous chemical studies of these elements in the solutions containing diverse complexing agents was developed in Joint Institute for Nuclear Research (JINR), Dubna . The procedure involves isolation and separation of target products on a series of ion-exchange columns. Since the production cross- -section of element 114 is low and the half-lives of its isotopes are short, the choice of correct sorbents is of particular importance for this issue. The 212 Pb isotope emits γ-rays, that gives the possibility of promising monitoring of its sorption on various sorbents . The
2 164 B. Kubica mechanisms of lead(ii) sorption on Dowex-1, Dowex-50 have been already examined [1, 27, 28]. Hitherto, there are a few publications dealing with the sorption of lead(ii) on transition metal hexacyanoferrates(ii) [4, 5, 9]. Therefore, searching for efficient sorbent for the lead(ii) sorption and establishing the best conditions for that process was our objective. Because recent investigation on the sorption of lead(ii) on transition metal hexacyanoferrates(ii) provided coherent results (K d >1000 cm 3 g 1 ) , we have decided to test the composite sorbents CuNCFM or NiNCFM, containing either copper(ii)-potassium hexacyanoferrate or nickel(ii)-potassium hexacyanoferrate and magnetite in the resin matrix. The sorptions was performed from hydrochloric, nitric and sulphuric acids solutions in the concentrations range from 10 4 mol dm 3 to 1 mol dm 3. The analytical distribution coefficients for the lead(ii) sorptions have been also evaluated. Methods Preparation of copper-potassium and nickel-potassium hexacyanoferrates An insoluble hexacyanoferrates exhibit a diversity in composition and structure what strongly depends on the way of preparation [2, 7, 10 12]. In our tests, the insoluble hexacyanoferrates were obtained by precipitation from a mixture of 660 cm 3 of 0.1 M K 4 Fe(CN) 6 with 1000 cm 3 CuCl 2 or NiCl 2. The molar ratio of divalent cations to ferrocyanide ions was 1.5:1. Then, the solutions were stirring for 2 h. After 48 h, the particles were washed with distillated water and separated by decantation. The precipitate was washed with water and dried in air at room temperature and then sieved. In the experiments, the hexacyanoferrate sorbents fractions between 0.12 mm and 0.2 mm were used. Chemical analysis For the determination of cations in complexes of hexacyanoferrates, the samples were decomposed with sulphuric acid and heated to dryness twice. The dried samples were leached with 0.1 M HCl and analyzed for K, Co, Cu, Zn, Ni, Fe using an atomic absorption spectrometry (AAS) technique. The total water content was determined by thermogravimetry. Morphology Scanning electron microscopy (SEM) was used to characterize the morphology of hexacyanoferrates. The samples were examined by SEM-5440 with an X-ray analyzer type LINK ISIS-300. Infrared (IR) spectroscopy Infrared spectra were recorded in the range cm 1 on samples dispersed in KBr. The samples were examined by a Bio-Rad FTS60v IR spectrometer. Powder X-ray diffraction X-ray diffraction patterns were recorded using PHILIPS X Pert APD (with a generator PW 1870 and a perpendicular goniometer PW 3020). CuK α X-ray radiation was used. Identification of CuNF and NiNF was made by reference to the database sets 1 49, Folder Diffraction File 1997 (International Centra for Diffraction Data, 12 Campus Boulevard). Preparation of composite sorbents The composite sorbents, CuNCFM and NiNCFM containing copper(ii)-potassium hexacyanoferrate(ii) or nickel(ii)-potassium hexacyanoferrate, magnetite and the sulphonated phenolic resin have been examined. The method of preparation of composite sorbents, MeNCF, containing the transition metal(ii)-potassium hexacyanoferrates(ii) and the sulphonated phenolic resin was developed and patented by Narbutt et al. . In the Institute of Nuclear Physics in Kraków that method was also modified and patented . The latter method has been used to prepare the loaded composite sorbents with magnetite, MeNCFM. These composite sorbents consist of the resin which serves as a matrix for a powdered mixture of chosen hexacyanoferrate(ii) and magnetite. The resin was synthesized by polycondensation of sulphonated phenol and formaldehyde [6, 21]. CuNCFM and NiNCFM were obtained by incorporation of the powdered mixture of magnetite and copper(ii)-potassium hexacyanoferrate(ii) or nickel(ii) hexacyanoferrate during formation of the resin matrix . In order to study the effect of the resin and magnetite on the sorption properties of copper(ii)- -potassium hexacyanoferrate and nickel(ii)-potassium hexacyanoferrate, the sorbent containing only the resin RLM (sulphonated phenol-formaldehyde resin with magnetite) was loaded with magnetite. Radionuclides The no-carrier-added radionuclides of 212 Pb were obtained by an emanation method from the system involving a column packed with Th(C 2 O 4 ) 2 2H 2 O. The description of the operation of the system and its outlook was already presented . Determination of the distribution coefficients Distribution coefficient, K d, is defined as the ratio of the given element concentration in the sorbent to the concentration of that element in a solution at equilibrium. The K d values for sorption of the 212 Pb isotope were determined in batch experiments where 0.03 g of the examined sorbent was mixed with 3 cm 3 of inorganic acid solution containing the radioisotope. The concentrations of the acid solutions varied in the range from 10 4 to 10 1 mol dm 3. Then, the samples were centrifuged for 15 min (4000 rpm) and thereafter a volume of 1 cm 3 was taken from each sample due to gamma activity measurement. The activity of these samples was compared with
3 Sorption of lead(ii) on copper(ii) and nickel-potassium hexacyanoferrates and magnetite-loaded Table 1. The composition of NiNF and CuNF Formula Ni (%) Cu (%) Zn (%) Co (%) Fe (%) K (%) NiNF CuNF Table 2. The composition of tested hexacyanoferrates Formula The composition of tested mixtures of hexacyanoferrates Structure The percentage composition of tested hexacyanoferrates K 0.32 Cu 1.91 [Fe(CN) 6 ] 3.1H 2 O K 2 Cu[Fe(CN) 6 ] Cubic 15% Cu 2 [Fe(CN) 6 ] 2H 2 O Cubic 80% KCu[Fe(CN) 6 ] 3.1H 2 O Tetragonal 5% K 1.24 Ni [Fe(CN) 6 ] 3H 2 O K 2 Ni[Fe(CN) 6 ] 1.5H 2 O Cubic 60% Ni 2 [Fe(CN) 6 ] 6H 2 O Cubic 35% KNi[Fe(CN) 6 ] Cubic 5% the activity of the standard (1 cm 3 ) that was sampled before performing the lead(ii) sorption. The gamma activity of the samples was measured using the a resolution gamma-spectrometer with a coaxial HPGe detector. The measurements were performed in 2π geometry. Taking into consideration the respectively short half-life of 212 Pb isotope ([T 1/2 = 10.64±0.01 h, E γ = kev, (43.3%)] ), we performed all the experiments within the same time period and at room temperature. The analytical distribution coefficients were evaluated using well-described algorithm . Sorption and desorption The desorption of lead(ii) was studied using a column technique. The columns with a diameter of 4 mm were filled with MeNCFM. The packed height was 2.5 cm. In order to perform the lead(ii) sorption, a volume of 100 cm 3 of chosen, inorganic acid solution (10 2 mol dm 3 ) containing no-carrier-added isotope 112 Pb was passed through the column using a peristaltic pump. After a lapse over 30 min, the elution was started at a flow rate of 1 cm 3 min 1. The solution of the same acid as that used for the sorption but at a concentration of 1 mol dm 3 was used as the eluent. In order to test whether the lead(ii) desorption occurs at the acid concentration chosen for performing the lead(ii) sorption, the gamma activity of the effluent collected during the sorption course was measured. These experiments were run with all the acids tested. holes. The sizes of the spherical sorbent grains ranged in diameter from 0.1 to 0.25 mm. The K d values for the sorption of lead(ii) on CuNCFM from the media of hydrochloric, sulphuric and nitric acids are presented in Figs. 1, 2 and 3, respectively. In order to elucidate the mechanism of the lead(ii) sorption on CuNCFM, the sorption run on RLM was shown as the control. It is seen from Figs. 1 3 that in the acid concentrations range from 10 4 to 10 2 mol dm 3 the K d values are relatively high, K d > 1000 cm 3 g 1, both for lead(ii) sorption on CuNCFM and on RLM. Together with increasing solution acidity, in the ph range from 4 to 2, the K d values are the highest. In all examined solutions, the sorption run on CuNCFM is similar to that on RLM what suggests that the mechanisms of lead(ii) sorption on both tested sorbents are identical in the acidic environment. On the other hand, in the chosen range of acid concentrations, the K d values for the lead(ii) sorption on CuNCFM are higher than those on RLM indicating that copper(ii)-potassium hexacyanoferrate(ii) contrib- Results and discussion Results of chemical analysis: AAS the obtained values of cations content are showed in Table 1; termogravimetry total content of water in complexes of hexacyanoferrates; X-ray diffraction analysis and IR confirm our hypothesis that hexacyanoferrates (description above) were the mixture of compounds; these mixtures contained at least three insoluble hexacyanoferrates of Ni or Cu where Fe in the hexacyano group was either in (II) and (III) oxidation state (see Table 2). The structure of sorbents seems to be an amorphous and crystalline mixture. Tested hexacyanoferrates were very heterogeneous exhibiting full of pores, vessels and Fig. 1. Distribution coefficients, K d, for lead(ii) sorption on the sorbents: CuNCFM and RLM from hydrochloric acid.
4 166 B. Kubica Fig. 2. Distribution coefficients, K d, for lead(ii) sorption on the sorbents: CuNCFM and RLM from sulphuric acid. Fig. 3. Distribution coefficients, K d, for lead(ii) sorption on the sorbents: CuNCFM and RLM from nitric acid. utes the sorption process. At an acid concentration of 10 1 mol dm 3, the values of K d sharply diminish for all the sorptions performed, see Figs Also we compared the obtained K d values with those for the lead(ii) sorption on Dowex-50 (see Ref. ). The comparison allowed to conclude that in nitric or sulphuric acid environment the general trend for the K d values changes is similar to that presented in Ref. . This suggests that under acidic conditions, the mechanism of lead(ii) sorption has an ion-exchange character. In the HCl range examined, Pb 2+ could form ions: Pb(Cl) + and Pb 2+, the latter being the main one [8, 17]. Hydrolysis of lead begins at upper ph = 5 and in this case, lead is not present as Pb(OH) + ions. Considering the lead(ii) sorption on CuNCFM, we took into account that the sorption occurs not only on copper(ii)-potassium hexacyanoferrate, but also on the resin-matrix. The lead(ii) sorption on the resin is described as ion- -exchange process in which sulphonic and phenolic groups are participating. One can find the evidence, in our former paper , where the comparison of the K d values for lead(ii) sorption on the resin and Dowex-50 from HCl medium in the same acidity range as that considered herein is given. In regard to the mechanism of lead(ii) sorption on hexacyanoferrates(ii) of transition metals, our explanation is based on the similarity in magnitude of ionic radii for potassium and lead(ii), 1.33 Å and 1.32 Å, respectively. This hypothesis was presented in Refs. [5, 29]. As far as magnetite is concerned there is a reason to believe that in the acidity range examined it does not reveal a tendency for sorption of the cations of lead(ii) [3, 18, 29]. An exception could be the case when ternary complexes of the type Fe sfc -anion-pb(ii) arise on the arise on the magnetite surface. It is seen from Fig. 1 that in the case of the lead(ii) sorption from hydrochloric acid the run of K d changes both on CuNCFM and on RLM differ from the sorption performed in the nitric and sulphuric acid media. The discrepancy is dealing with the fact that the evaluated K d values are surprisingly high both on CuNCFM and on RLM at hydrochloric acid concentration of 10 2 mol dm 3. It is clear from the comparison made in Figs. 1 3 that the chlorine anions affect the sharp growth of the K d values at the indicated acid concentration. Observed phenomena could be explained by Cl affinity to Fe 3+ and Pb 2+ in aqueous solution. Cl (aq) readily forms complexes with Fe 3+ (aq) (Log [K fm,fecl2 +] = 1.45) and Pb 2+ (aq) (Log [K fm,pbcl + = 1.6]) . Thus, it would be reasonable to suggest that a ternary surface complexes, Fe scf -Cl-Pb(II), are formed on the magnetite surface. The possibility of complex formation was reported in Ref. . Although this explanation seems to be reasonable, the question why it occurs at the indicated acid concentration still remains to be examined. Coming back to Figs. 1, 2 and 3, it is shown that in all the media examined a distinct drop of the values of K d occurs at an acid concentration of 10 1 mol dm 3. It is safe to assume that during the sorption process, the H + ions delivered into the solution by adding acid at this concentration become quite competitive with lead(ii). The lead sorption from hydrochloric acid on CuNF, NiNF (copper(ii)-potassium hexacyanoferrate(ii) CuNF and nickel(ii)-potassium hexacyanoferrate NiNF) and respectively on CuNCFM, NiNCFM were compared and the results were shown in Fig. 4. In the tested acid concentrations, the K d values for the lead(ii) sorption on CuNCFM and NiNCFM are higher than those on CuNF and NINF suggesting that the resin makes a contribution to the sorption process. It seems that lead sorption performed on CuNF is more efficient than on NiNF, however, the values of K d of lead(ii) ions on CuNCFM and NiNCFM are equal to each other. The Pb 2+ desorption on CuNCFM from nitric, hydrochloric and sulphuric acids has also been studied
5 Sorption of lead(ii) on copper(ii) and nickel-potassium hexacyanoferrates and magnetite-loaded Fig. 4. Distribution coefficients, K d, for lead(ii) sorption on the sorbents: CuNF and NiNF (a) and on the sorbents: CuNCFM and NiNCFM from hydrochloric acid (b). under dynamic conditions using column technique. The desorption percent values were 99, 98 and 91% in HCl, H 2 SO 4 and HNO 3, respectively, and the volume of every effluent about 3 cm 3. The desorption curves for the processes performed with the tested eluents are presented in Fig. 5. To compare desorption curves, we expressed the activity of eluates in relative units (cm). The results showed in Fig. 4 indicate that the desorptions performed in hydrochloric and sulphuric acids, run in a similar manner. Opposite to HCl and H 2 SO 4, the desorption curve performed in nitric acid differs significantly. Since the desorption percent value for nitric acid conditions is rather high (91%), the discrepancy is likely dealing with much slower kinetics of the process. Thus, the chosen flow rate (1 cm 3 min 1 ) and the concentration (1 mol dm 3 ) seems to be incorrect for this eluent. Moreover, from some point of the desorption course, the eluate activity began to decline unevenly (see desorption curves for HCl and HNO 3 ). This might be a hint for other explanation of the lead(ii) sorption-desorption mechanism that accompanies the ion-exchange on copper(ii)-potassium hexacyanoferrate(ii) and exhibits its own kinetics. The observed desorption curves asymmetry also confirm this interpretation, whereas the similarity in Pb 2+ desorption has been studied under dynamic conditions on NiNF, NiNCF and resin only in hydrochloric acid. The lead desorption from NiNF is widely described in publication . The desorption percent obtained for NiNF was 73%, opposite to NiNCF for which the lead(ii) desorption rate is very slow . To conclude, in given conditions, the lead(ii) sorption process was complex including the sorption either on copper(ii)-potassium hexacyanoferrate, nickel(ii)- -potassium hexacyanoferrate or on the resin. Conclusions The preliminary data for the lead(ii) sorption on these sorbents showed that in the case of the sorption performed in the sulphuric and nitric acid solutions the slight increase of the K d values with the growth of the acid concentration up to 10 2 mol dm 3 was observed; this is true for the sorption either on CuNCFM or on RLM. However, the K d values sharply increased at an acid in concentration of 10 2 mol dm 3. The explanation of this fact remains to be confirmed by further studies. In medium acidity of ph = 1, the K d values sharply decrease what is observed for all the systems tested. To summarize, the optimum conditions for the sorption of the trace amounts of the no-carrier-added 212 Pb isotope on the copper(ii)-potassium hexacyanoferrate, nickel(ii)-potassium hexacyanoferrate and on RLM in the acid concentration range from mol dm 3. Thus, the lead(ii) sorption is efficient both under static and dynamic conditions in the whole tested range of acid concentrations. The sorbent, CuNCFM is found to be stable under conditions examined. The desorption percent values of more than 90% have been obtained for the acids, and hydrochloric acid is the most suitable medium for performing the lead(ii) sorption- -desorption on CuNCFM and on NiNCFM, where at its concentration of 10 2 mol dm 3 the K d is the highest (K d 10,000 cm 3 g 1 ) and efficient desorption occurs at an acid concentration of 1 mol dm 3. Acknowledgment. The author thanks Mrs M. Tuteja- -Krysa and Mrs H. Godunova for technical assistance. References Fig. 5. Comparison of the elutions performed from the different acid media. 212 Pb was eluted from the composite sorbent, CuNCFM. A concentration of all the eluents was of 1 mol dm Abollino O, Aceto M, Sarzanini C, Mentasti E (2000) The retention of metal species by different solid sorbents: mechanisms for heavy metal speciation by sequential three column uptake. Anal Chim Acta 411: Ayrault A, Loos-Neskovic C, Fedoroff M, Garnier E (1994) Copper hexacyanoferrates: preparation, composition and structure. Talanta 41: Bargar JR, Brown GE Jr, Parks GA (1998) Surface complexation of Pb(II) at oxide-water interfaces: III.
6 168 B. Kubica XAFS determination of Pb(II) and Pb(II)-chloro adsorption complexes on goethite and alumina. Geochim Cosmochim Acta 62: Jain AK, Singh RP, Bala C (1985) Preparation and ion- -exchange properties of stannic hexacyanoferrate(iii). Chem Anal (Warsaw) 30: Kubica B, Godunowa H, Tuteja-Krysa M, Stobiński M, Misiak R (2004) Sorption of lead(ii) on transition metal hexacyanoferrates(ii) and on nickel(ii)-potassium hexacyanoferrate(ii) resin composite in hydrochloric acid medium. J Radioanal Nucl Chem 262: Kubica B, Szeglowski Z, Tuteja-Krysa M, Fiałkowski R (2001) Pol Pat no P Kubica B, Tuteja-Krysa M, Misiak R et al. (2003) The behavior of Ba and Sr on inorganic and organic ion- -exchangers from sulphuric acid solutions. Preliminary experiments. J Radioanal Nucl Chem 258: Liu Qi, Liu Y (2003) Distribution of Pb(II) species in aqueous solutions. J Colloid Interface Sci 268: Lizalova B, Szeglowski Z, Zvara I, Timokhin SN, Tronh thi Thu My (2003) Determination of a thorium content in soil samples by means of gamma-activation analysis and X-ray spectrometry. In: The Flerov Laboratory of Nuclear Reaction Scientific Report Dubna, pp Loos-Neskovic C, Fedoroff M (1989) Fixation mechanisms of cesium on nickel and zinc ferrocyanides. Solv Extr Ion Exch 7: Loos-Neskovic C, Fedoroff M, Garnier E, Gravereau P (1984) Zinc and nickel ferrocyanides: preparation, composition and structure. Talanta 31: Loos-Neskovic C, Fedoroff M, Gravereau P (1989) Prepa- ration, composition and structure of some nickel and zinc ferrocyanides: experimental results. Talanta 36: Lurie J (1965) Handbook of analytical chemistry. Mir 13. Publishers, Moscow 14. Magill J (2003) An integrated environment for computations on radionuclides and their radiation. Springer, Heidelberg 15. Narbutt J, Bartoś B, Bilewicz A, Szeglowski Z (1988) Pol Pat no ; (1988) US Patent no ; (1991) Eur Pat no Oganessian YuTs, Utyonkov VK, Lobanov YuV et al. (2001) Synthesis of heavy elements, observation of the decay of In: JINR Report JINR, Dubna, pp Polanskij NG (1986) Analytical chemistry of elements; lead Pb. Science, Moscow, p Potter HAB, Yong RN (1999) Influence of iron/aluminium ratio on the retention of lead and copper by amorphous iron-aluminium oxides. Appl Clay Sci 14: Pyper NC, Grant IP (1981) Theoretical chemistry of the 7p series superheavy elements. I. Atomic structure studied by multi-configuration Dirac-Fock theory. Proc Royal Soc A 376: Pyykkö P (1988) Relativistic effects in structural chem- 20. istry. Chem Rev 88: Rabek TI (1960) The theoretical basis for the synthesis of polyelectrolytes. Państwowe Wydawnictwo Naukowe, Warsaw 22. Smolańczuk R (1997) Properties of the hypothetical spherical superheavy nuclei. Phys Rev C 56: Szeglowski Z (2003) Model experiments on chemical properties of super heavy elements in aqueous solutions. Acta Phys Pol B 34: Szeglowski Z, Bruchertseifer H, Domanov VP et al. (1990) Study of the solution chemistry of the element 104-Kurchatovium. Radiochim Acta 51: Szeglowski Z, Constatinescu O, Hussonnois M (1994) Sorption behaviour of some I to V group elements on nickel hexacyanoferrate(ii) composite ion exchanger. Radiochim Acta 64: Szeglowski Z, Kubica B, Din Thi Lien et al. (2005) A 212 Pb generator for model experiments on aqueous chemistry of element 114. J Radioanal Nucl Chem 265: van Erkelens PC (1961) On the concentration and separa- tion of the trace elements: Fe, Cu, Zn, Mn, Pb, Mo and Co: ion exchange methods. Anal Chim Acta 25:42 50 Warhol M (1982) Ion exchangers in analytical chemistry. 28. Academia, Prague, p Yamaguchi NU, Okazaki M (2002) Micro volume changes due to Pb(II) and Cu(II) sorption on amorphous Fe(III) hydroxide. J Colloid Interface Sci 249: Zielińska B, Bilewicz A (2005) Influence of relativistic effects on hydrolysis of Ra 2+. J Radioanal Nucl Chem 266: